#------------------------------------------------------------------------------
#$Date: 2016-02-21 02:03:34 +0200 (Sun, 21 Feb 2016) $
#$Revision: 176798 $
#$URL: svn://www.crystallography.net/cod/cif/2/23/59/2235962.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2235962
loop_
_publ_author_name
'Sologub, Oksana'
'Michiue, Yuichi'
'Mori, Takao'
_publ_section_title
;
 Boron carbide, B₁₃₋ₓC2-y (x = 0.12, y =
 0.01)
;
_journal_coeditor_code           RU2039
_journal_issue                   8
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i67
_journal_paper_doi               10.1107/S1600536812033132
_journal_volume                  68
_journal_year                    2012
_chemical_formula_iupac          'C1.99 B12.88'
_chemical_formula_moiety         'C1.99 B12.88'
_chemical_formula_sum            'C1.99 B12.88'
_chemical_formula_weight         163.137
_chemical_name_systematic
;
Boron carbide
;
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.6530(8)
_cell_length_b                   5.6530(8)
_cell_length_c                   12.156(4)
_cell_measurement_reflns_used    20
_cell_measurement_temperature    293
_cell_measurement_theta_max      50
_cell_measurement_theta_min      8
_cell_volume                     336.42(13)
_computing_cell_refinement
'Rigaku/AFC Diffractometer Control Software (Rigaku, 1998)'
_computing_data_collection
'Rigaku/AFC Diffractometer Control Software (Rigaku, 1998)'
_computing_data_reduction
'TEXSAN (Molecular Structure Corporation, 1998)'
_computing_molecular_graphics    'ATOMS (Dowty, 1999)'
_computing_publication_material
'SHELXL97 (Sheldrick, 2008) and WinGX (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_measurement_device_type  'Rigaku AFC 7R'
_diffrn_measurement_method       ω-2θ
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1508
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            1489
_diffrn_reflns_theta_full        39.83
_diffrn_reflns_theta_max         39.83
_diffrn_reflns_theta_min         4.49
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 150
_diffrn_standards_interval_time  105
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    0.097
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.416
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             229
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.21
_refine_diff_density_max         0.554
_refine_diff_density_min         -0.374
_refine_ls_goodness_of_fit_ref   1.031
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         284
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.029
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0481P)²+0.3407P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.1087
_reflns_number_gt                184
_reflns_number_total             284
_reflns_threshold_expression     I>2sigma(I)
_cod_data_source_file            ru2039.cif
_cod_data_source_block           I
_cod_original_cell_volume        336.42(17)
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               2235962
_cod_database_fobs_code          2235962
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'y, x, -z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'-y, -x, z'
'x-y, x, -z'
'x, x-y, z'
'-x+y, y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'x+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
B B1 0.44092(16) 0.55908(16) 0.05298(12) 0.0053(3) Uani 0.958(4)
C C11 0.44092(16) 0.55908(16) 0.05298(12) 0.0053(3) Uani 0.042(4)
B B2 0.50336(16) 0.49664(16) 0.19232(11) 0.0054(3) Uani 1
B B3 0 0 0 0.0118(8) Uani 0.87
C C1 0 0 0.1177(5) 0.0071(8) Uani 0.87(2)
B B11 0 0 0.079(4) 0.0071(8) Uani 0.13(2)
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
C11 B1 B1 19_665 19_665 0.00(8)
C11 B1 B2 19_665 . 118.22(14)
B1 B1 B2 19_665 . 118.22(14)
C11 B1 B2 19_665 28 121.45(8)
B1 B1 B2 19_665 28 121.45(8)
B2 B1 B2 . 28 59.01(5)
C11 B1 B2 19_665 26_455 121.45(8)
B1 B1 B2 19_665 26_455 121.45(8)
B2 B1 B2 . 26_455 59.01(5)
B2 B1 B2 28 26_455 105.68(11)
C11 B1 B1 19_665 4_565 125.36(8)
B1 B1 B1 19_665 4_565 125.36(8)
B2 B1 B1 . 4_565 107.10(6)
B2 B1 B1 28 4_565 107.02(6)
B2 B1 B1 26_455 4_565 59.72(5)
C11 B1 C11 19_665 4_565 125.36(8)
B1 B1 C11 19_665 4_565 125.36(8)
B2 B1 C11 . 4_565 107.10(6)
B2 B1 C11 28 4_565 107.02(6)
B2 B1 C11 26_455 4_565 59.72(5)
B1 B1 C11 4_565 4_565 0.00(9)
C11 B1 C11 19_665 2_665 125.36(8)
B1 B1 C11 19_665 2_665 125.36(8)
B2 B1 C11 . 2_665 107.10(6)
B2 B1 C11 28 2_665 59.72(5)
B2 B1 C11 26_455 2_665 107.02(6)
B1 B1 C11 4_565 2_665 60
C11 B1 C11 4_565 2_665 60
C11 B1 B1 19_665 2_665 125.36(8)
B1 B1 B1 19_665 2_665 125.36(8)
B2 B1 B1 . 2_665 107.10(6)
B2 B1 B1 28 2_665 59.72(5)
B2 B1 B1 26_455 2_665 107.02(6)
B1 B1 B1 4_565 2_665 60
C11 B1 B1 4_565 2_665 60
C11 B1 B1 2_665 2_665 0.00(10)
C1 B2 B11 25 25 15.1(12)
C1 B2 B2 25 26_455 121.49(7)
B11 B2 B2 25 26_455 125.0(2)
C1 B2 B2 25 28 121.49(7)
B11 B2 B2 25 28 125.0(2)
B2 B2 B2 26_455 28 108.39(8)
C1 B2 B1 25 . 119.9(2)
B11 B2 B1 25 . 135.0(14)
B2 B2 B1 26_455 . 60.73(7)
B2 B2 B1 28 . 60.73(7)
C1 B2 C11 25 28 121.07(19)
B11 B2 C11 25 28 108.5(11)
B2 B2 C11 26_455 28 108.78(7)
B2 B2 C11 28 28 60.26(7)
B1 B2 C11 . 28 110.05(9)
C1 B2 B1 25 28 121.07(19)
B11 B2 B1 25 28 108.5(11)
B2 B2 B1 26_455 28 108.78(7)
B2 B2 B1 28 28 60.26(7)
B1 B2 B1 . 28 110.05(9)
C11 B2 B1 28 28 0.00(11)
C1 B2 C11 25 26_455 121.07(19)
B11 B2 C11 25 26_455 108.5(11)
B2 B2 C11 26_455 26_455 60.26(7)
B2 B2 C11 28 26_455 108.78(7)
B1 B2 C11 . 26_455 110.05(9)
C11 B2 C11 28 26_455 60.56(11)
B1 B2 C11 28 26_455 60.56(11)
C1 B2 B1 25 26_455 121.07(19)
B11 B2 B1 25 26_455 108.5(11)
B2 B2 B1 26_455 26_455 60.26(7)
B2 B2 B1 28 26_455 108.78(7)
B1 B2 B1 . 26_455 110.05(9)
C11 B2 B1 28 26_455 60.56(11)
B1 B2 B1 28 26_455 60.56(11)
C11 B2 B1 26_455 26_455 0.00(4)
B11 B3 B11 . 19 180.0000(10)
B11 B3 C1 . 19 180.0000(10)
B11 B3 C1 19 19 0.0000(10)
B11 B3 C1 . . 0.0000(10)
B11 B3 C1 19 . 180.0000(10)
C1 B3 C1 19 . 180
B3 C1 B2 . 25 100.1(2)
B3 C1 B2 . 26_455 100.1(2)
B2 C1 B2 25 26_455 117.01(13)
B3 C1 B2 . 28_445 100.1(2)
B2 C1 B2 25 28_445 117.01(13)
B2 C1 B2 26_455 28_445 117.01(13)
B3 B11 B2 . 25 115.2(13)
B3 B11 B2 . 26_455 115.2(13)
B2 B11 B2 25 26_455 103.2(16)
B3 B11 B2 . 28_445 115.2(13)
B2 B11 B2 25 28_445 103.2(16)
B2 B11 B2 26_455 28_445 103.2(16)
B3 B11 B11 . 19 0.0000(10)
B2 B11 B11 25 19 115.2(13)
B2 B11 B11 26_455 19 115.2(13)
B2 B11 B11 28_445 19 115.2(13)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
B1 C11 19_665 1.731(3)
B1 B1 19_665 1.731(3)
B1 B2 . 1.801(2)
B1 B2 28 1.8091(15)
B1 B2 26_455 1.8091(15)
B1 B1 4_565 1.825(3)
B1 C11 4_565 1.825(3)
B1 C11 2_665 1.825(3)
B1 B1 2_665 1.825(3)
B2 C1 25 1.6239(19)
B2 B11 25 1.77(2)
B2 B2 26_455 1.7778(17)
B2 B2 28 1.7778(17)
B2 C11 28 1.8091(15)
B2 B1 28 1.8091(15)
B2 C11 26_455 1.8091(15)
B2 B1 26_455 1.8091(15)
B3 B11 . 0.96(5)
B3 B11 19 0.96(5)
B3 C1 19 1.430(6)
B3 C1 . 1.430(6)
C1 B2 25 1.6239(19)
C1 B2 26_455 1.6239(19)
C1 B2 28_445 1.6239(19)
B11 B2 25 1.77(2)
B11 B2 26_455 1.77(2)
B11 B2 28_445 1.77(2)
B11 B11 19 1.92(9)
